Upload
others
View
42
Download
0
Embed Size (px)
Citation preview
Optical Properties of Solids: Lecture 6
Stefan ZollnerNew Mexico State University, Las Cruces, NM, USA
and Institute of Physics, CAS, Prague, CZR (Room 335)[email protected] or [email protected]
NSF: DMR-1505172http://ellipsometry.nmsu.edu
These lectures were supported by • European Union, European Structural and Investment Funds (ESIF) • Czech Ministry of Education, Youth, and Sports (MEYS), Project IOP
Researchers Mobility – CZ.02.2.69/0.0/0.0/0008215
Thanks to Dr. Dejneka and his department at FZU.
Optical Properties of Solids: Lecture 5+6Lorentz and Drude model: Applications1. Metals, doped semiconductors2. InsulatorsSellmeier equation, Poles, Cauchy dispersionAnalytical properties of ε
Al
NiO
New Mexico State University
References: Dispersion, Analytical Properties
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 3
Standard Texts on Electricity and Magnetism:• J.D. Jackson: Classical Electrodynamics• L.D. Landau & J.M. Lifshitz, Vol. 8: Electrodynamics of Cont. Media
Ellipsometry and Polarized Light:• R.M.A. Azzam and N.M. Bashara: Ellipsometry and Polarized Light• H.G. Tompkins and E.A. Irene: Handbook of Ellipsometry
(chapters by Rob Collins and Jay Jellison)• H. Fujiwara, Spectroscopic Ellipsometry• Mark Fox, Optical Properties of Solids• H. Fujiwara and R.W. Collins: Spectroscopic Ellipsometry for PV (Vol 1+2)• Zollner: Propagation of EM Waves in Continuous Media (Lecture Notes)• Zollner: Drude and Kukharskii mobility of doped semiconductors extracted
from FTIR ellipsometry spectra, J. Vac. Sci. 37, 012904 (2019).
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 4
Drude-Lorentz Model: Free and Bound Charges
𝐸𝐸 𝑡𝑡 = 𝐸𝐸0 exp −𝑖𝑖𝑖𝑖𝑡𝑡
qq qx
qE
bv
v
𝐸𝐸 𝑡𝑡 = 𝐸𝐸0 exp −𝑖𝑖𝑖𝑖𝑡𝑡
𝜀𝜀 𝑖𝑖 = 1 −�𝑖𝑖
𝑖𝑖𝑃𝑃,𝑖𝑖2
𝑖𝑖2 + 𝑖𝑖𝛾𝛾𝐷𝐷,𝑖𝑖𝑖𝑖+ �
𝑖𝑖
𝐴𝐴𝑖𝑖𝑖𝑖0,𝑖𝑖2
𝑖𝑖0,𝑖𝑖2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾0,𝑖𝑖𝑖𝑖
ωP (unscreened) plasma frequency of free chargesω0 resonance frequency of bound chargesγD, γ0 broadenings of free and bound chargesA amplitude of bound charge oscillations (density, strength)
𝑖𝑖𝑃𝑃2 =
𝑛𝑛𝑓𝑓𝑒𝑒2
𝑚𝑚𝜀𝜀0Discuss plasma frequency trends.
Lorentz:Bound Charges
Drude:Free Charges
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 5
Drude-Lorentz Model: Free and Bound Charges
𝜀𝜀 𝑖𝑖 = 1 −�𝑖𝑖
𝑖𝑖𝑃𝑃,𝑖𝑖2
𝑖𝑖2 + 𝑖𝑖𝛾𝛾𝐷𝐷,𝑖𝑖𝑖𝑖+ �
𝑖𝑖
𝐴𝐴𝑖𝑖𝑖𝑖0,𝑖𝑖2
𝑖𝑖0,𝑖𝑖2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾0,𝑖𝑖𝑖𝑖
Semiconductors
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 6
Free-Carrier Reflection in doped semiconductors
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 7
Fox, Optical Properties of Solids
Doped semiconductors behave just like a metal, except for the lower carrier density; plasma frequency in infrared region.
Carrier density in m-3
InSb
Reflectance minimum near plasma frequency
𝑖𝑖𝑃𝑃2 =
𝑛𝑛𝑓𝑓𝑒𝑒2
𝑚𝑚∗𝑚𝑚0𝜀𝜀0
Infrared ellipsometry of doped semiconductors
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 8
Doped semiconductors behave just like a metal, except for the lower carrier density; plasma frequency in infrared region.Only visible for electrons (small mass).
Wave Number (cm-1)0 100 200 300 400 500 600
Ψ in
deg
rees
0
10
20
30
40
50
Model Fit Exp AnE 60°Exp AnE 70°Exp AnE 80°
Wave Number (cm-1)0 100 200 300 400 500 600
Ψ in
deg
rees
0
10
20
30
40
50
Model Fit Exp AnE 60°Exp AnE 70°Exp AnE 80°
Drude
Drude
TO/LO TO/LO
n-type InAsm=0.027n=6.3×1016 cm−3
γ=50 cm−1
µ=6800 cm2/Vs
n-type GaSb:Tem=0.13 (?!?)n=1.3×1017 cm−3
γ= 71 cm−1
µ=1000 cm2/Vs
𝜀𝜀 𝑖𝑖 = 1 −𝑖𝑖𝑃𝑃2
𝑖𝑖2 + 𝑖𝑖𝛾𝛾𝑖𝑖
Abadizaman, Emminger, Knight, Schubert
Infrared ellipsometry of doped semiconductors
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 9
Doped semiconductors behave just like a metal, except for the lower carrier density; plasma frequency in infrared region.
𝜀𝜀 𝑖𝑖 = 1 −𝑖𝑖𝑃𝑃2
𝑖𝑖2 + 𝑖𝑖𝛾𝛾𝑖𝑖
30 meV lower cut-off insufficient to see Drude term.
Plasmon effect:Doping pushes LO phonon to higher energies.
Drude TO/LO
Zollner, JVSTB 37, 012904 (2019)
Optical Hall Effect: Ellipsometry with magnetic field
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 10
If we measure Mueller matrix spectra in a magnetic field, we get carrier concentrations, mobilities, effective masses.
Abadizaman, Emminger, Knight, Schubert
m=0.027n=6.3×1016 cm−3
γ=50 cm−1
µ=6800 cm2/Vs
m=0.13 (?!?)n=1.3×1017 cm−3
γ= 71 cm−1
µ=1000 cm2/Vs
Multi-valley semiconductors
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 5 11
GaSb is a direct semiconductor (like GaAs), but ALMOST indirect.The L-valley in GaSb is only 80 meV above the Γ-valley.Almost all electrons are in the L-valley at room temperature.
kBT=26 meVEΓ=730 meVEffective massesmΓ=0.041mL
⊥=0.11mL
||=0.954 L-valleysmL
DOS=0.57mtransport=
We need a model with two carrier species, one of them anisotropic.Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 11
Multiple Drude Contributions
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 12
• Electron mass depends on orbital (s, p, d, f)s: light (small mass m*<<1)p: intermediate (m*~0.3 to 1)d,f: heavy (large mass m*>>1)p,d,f: usually anisotropic
• Electrons and holes
• Different CB minima (Γ,L,X)
• Different VB hole bands (light, heavy, split-off)
P. Drude, Phys. Z. 1, 161 (1900).
VB: Valence band (filled)
CB: Conduction band (empty)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 13
𝜀𝜀 𝑖𝑖 = 1 −𝑖𝑖𝑃𝑃2
𝑖𝑖2 + 𝑖𝑖𝛾𝛾𝑖𝑖
𝑖𝑖𝑃𝑃2 =𝑛𝑛𝑞𝑞2
𝑚𝑚𝜀𝜀0 Charge density
Drude Model for Anisotropic Free Carriers
Conduction band minima in Ge and Siare anisotropic. Ge: ml=1.59, mt=0.0815.
Ener
gy (e
V)
Valence band maxima in semiconductors are warped (Luttinger parameters).
E k =ℏ2k2
2m
m−1 =1ℏ2𝜕𝜕2E k𝜕𝜕k2
=ml−1 0 00 mt
−1 00 0 mt
−1
m =𝑚𝑚𝑙𝑙𝑚𝑚𝑡𝑡
𝑚𝑚𝑡𝑡 + 2𝑚𝑚𝑙𝑙Drude formula still valid, but ε, ωp
2, m−1, and γ are tensors.
P. Drude, Phys. Z. 1, 161 (1900).
∆-valleyDrude mass
Harmonic mean
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 14
Grey α-tin is even more complicated
We need a model with THREE carrier species, one of them anisotropic.
L-electron light “hole”
heavy hole
Parabolic spherical bands
∆EΓL≈0
“electron”
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 15
Add strain and warping in Sn1-xGex alloys
How do we model Drude response of free carriers with realistic band structures?
Dirac point
Warping
Indirectgap
12 meV splitting(97 cm−1)
Direct gap
400 cm-1
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 16
Semiclassical Model of Electron DynamicsAshcroft & Mermin, Chapter 12
𝑟𝑟 = ��𝑣𝑛𝑛 𝑘𝑘 =ℏ𝑘𝑘𝑚𝑚
=1ℏ𝜕𝜕𝐸𝐸𝑛𝑛 𝑘𝑘𝜕𝜕𝑘𝑘
ℏ��𝑘 = 𝑞𝑞 𝐸𝐸 𝑟𝑟, 𝑡𝑡 + ��𝑣𝑛𝑛 𝑘𝑘 × 𝐵𝐵 𝑟𝑟, 𝑡𝑡
𝑓𝑓 𝐸𝐸𝑛𝑛 𝑘𝑘 =1
exp 𝐸𝐸𝑛𝑛 𝑘𝑘 − 𝐸𝐸𝐹𝐹 /𝑘𝑘𝐵𝐵𝑇𝑇 + 1
𝑚𝑚𝑐𝑐 𝐸𝐸, 𝑘𝑘𝑧𝑧 =ℏ2
2𝜋𝜋𝜕𝜕𝐴𝐴 𝐸𝐸, 𝑘𝑘𝑧𝑧
𝜕𝜕𝐸𝐸
“Electrons move along curves given by the intersection of surfaces of constant energy with planes perpendicular magnetic field.” Is there an optical analog to Shubnikov-de Haas effect? (Ge-Sn, GaSb)
How do we model Drude response of free carriers with realistic band structures?
Anisotropic masses (GaSb L-valley)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 17
Longitudinal mass at L ml=0.95Transverse mass at L mt=0.11
Density of states mass md=0.57(geometric mean)
Drude transport mass mD=0.15(harmonic mean)
Cyclotron mass
Dresselhaus, Dresselhaus, Cronin, Gomes, Solid-State Properties (10.50)
𝑚𝑚𝑐𝑐 =det𝑚𝑚𝑏𝑏 � 𝑚𝑚 � 𝑏𝑏
Optical Hall effect measurements on anisotropic materials are sparse. Need measurements on bulk Si, Ge, GaP with different orientations (change direction of magnetic field). How about SiC?
𝑚𝑚𝑑𝑑 =3𝑁𝑁𝑉𝑉2𝑚𝑚𝑙𝑙𝑚𝑚𝑡𝑡
2
3𝑚𝑚𝐷𝐷
=1𝑚𝑚𝑙𝑙
+2𝑚𝑚𝑡𝑡
Cyclotron Resonance
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 18
Measure microwave absorption as a function of the magnetic field.Information about VB warping.
Dresselhaus, Kip, Kittel, Phys. Rev. 98, 368 (1955)
ml=0.08
mt=1.58
B
𝑖𝑖𝑐𝑐 =𝑞𝑞𝐵𝐵𝑚𝑚
4 K, 24 GHz
10000 Oe=1 T
Insulators
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 19
Transparent region below the band gap (VIS/UV).
Forbidden “energy gap”.
Semiconductors are insulators with small band gap (IR).
Valence band filled.Conduction band empty.
Filled bands do not carry current.
VB: Valence band (filled)
CB: Conduction band (empty)
Multiple Lorentz Contributions: IR, UV, x-ray
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 20
IR: lattice vibrations
VIS/UV: valence electrons(usually broadened by band structure effects)
x-ray: core electrons
Amplitude depends on• Density of oscillators• Matrix elements• Born effective charge
Fox, Fig. 2.6
Multiple Lorentz Contributions: SiO2 as an Example
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 21
IR: lattice vibrations(Si-O bend, stretch)
VIS: Nothing happens
UV: valence electrons(interband transitions)
x-ray: core electrons(absorption edges)
Amplitude depends on• Density of oscillators• Matrix elements• Born effective charge
IRVIS
UV
x-ray
Fox, Fig. 2.7
Poles, Sellmeier Approximation
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 22
Set γ=0 far from resonance.Lorentz oscillator becomes a pole
Rewrite as a function of λ
Several Lorentz oscillators(one in IR, two in UV)
Sellmeier approximation.
𝜀𝜀 𝑖𝑖 = 1 +𝐴𝐴𝑖𝑖0
2
𝑖𝑖02 − 𝑖𝑖2
𝜀𝜀 𝜆𝜆 = 1 +𝐵𝐵𝜆𝜆2
𝜆𝜆2 − 𝐶𝐶
𝜀𝜀 𝜆𝜆 = 1 + �𝑖𝑖
𝐵𝐵𝑖𝑖𝜆𝜆2
𝜆𝜆2 − 𝐶𝐶𝑖𝑖
Fox, Fig. 2.10
The Cauchy equation
can be viewed as a Laurent series expansion ofthe Sellmeier equation
Comments:The Cauchy equation does not include absorption and therefore is not Kramers-Kronig consistent. Absorption is often included with an Urbach tail
but this still does not make it Kramers-Kronig consistent.Not recommended, use Tauc-Lorentz model instead.
Cauchy Equation (Urbach Tail)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 23
𝑛𝑛 𝜆𝜆 = 𝜀𝜀 𝜆𝜆 = 𝐴𝐴 +𝐵𝐵𝜆𝜆2
+𝐶𝐶𝜆𝜆4
𝑛𝑛 𝜆𝜆 = 𝜀𝜀 𝜆𝜆 = 1 +𝐵𝐵𝜆𝜆2
𝜆𝜆2 − 𝐶𝐶
𝑘𝑘 𝐸𝐸 = 𝛼𝛼𝑒𝑒𝛽𝛽 𝐸𝐸−𝛾𝛾
Insulator Phonon Spectra (Ge)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 24
Inelastic neutron scattering measures entire phonon dispersion.Optical experiments only probe k≈0, because λpa. Ge is IR-inactive (no dipole moment)
Neutron scattering
Fox, Fig. 10.2
Infrared Lattice Vibrations (Lorentz model)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 25
𝜀𝜀 𝑖𝑖 = 𝜀𝜀∞ + �𝑖𝑖
𝐴𝐴𝑖𝑖𝑖𝑖0,𝑖𝑖2
𝑖𝑖0,𝑖𝑖2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾0,𝑖𝑖𝑖𝑖
In polar materials (Born effective charge), TO and LO modes are split.TO: transverse optical (displacement perpendicular to k)LO: longitudinal optical (displacement along k)ε2 has peak at TO frequencyε1 is negative from TO to LO frequency (reflectance is 1)
Fox, Fig. 10.4
Infrared Lattice Vibrations (Lorentz model)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 26
In polar materials (Born effective charge), TO and LO modes are split.TO: transverse optical (atomic displacement perpendicular to k)LO: longitudinal optical (atomic displacement along k)ε2 has peak at TO frequencyε1 is negative from TO to LO frequency (reflectance is 1)Restrahlen band extends from TO to LO energy.
Fox, Fig. 10.5
ReststrahlenBand
𝜀𝜀 𝑖𝑖 = 𝜀𝜀∞ +𝐴𝐴𝑖𝑖0
2
𝑖𝑖02 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾0𝑖𝑖
Infrared Lattice Vibrations in GaP
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 27
ReststrahlenBand
ε∞=9.14ε0=15.7
364.9 cm-1
402.5 cm-1
Loss function
epsilon
psi
Delta
Infrared Lattice Vibrations (Lorentz model)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 28
Lyddane Sachs Teller relation (Lorentz model)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 29
𝜀𝜀s𝑖𝑖𝑇𝑇𝑇𝑇2 = 𝜀𝜀∞𝑖𝑖𝐿𝐿𝑇𝑇
2 LST relation
Lyddane, Sachs, Teller, Phys. Rev. 59, 673 (1941)
Lyddane Sachs Teller relation (Lorentz model)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 30
𝜀𝜀 𝑖𝑖 = 𝜀𝜀∞ +𝐴𝐴𝑖𝑖0
2
𝑖𝑖02 − 𝑖𝑖2
Lorentz model (γ=0) for one TO/LO phonon mode
At zero frequency (ω=0) define static dielectric constant εs
Define ωLO through ε(ωLO)=0(Longitudinal modes require ε=0).
or
𝜀𝜀s = 𝜀𝜀 𝑖𝑖 = 0 = 𝜀𝜀∞ + 𝐴𝐴
0 = 𝜀𝜀∞ +𝐴𝐴𝑖𝑖0
2
𝑖𝑖02 − 𝑖𝑖𝐿𝐿𝑇𝑇2
𝜀𝜀s𝑖𝑖𝑇𝑇𝑇𝑇2 = 𝜀𝜀∞𝑖𝑖𝐿𝐿𝑇𝑇
2 LST relation
Lyddane, Sachs, Teller, Phys. Rev. 59, 673 (1941)
Generalized Lyddane Sachs Teller relations
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 31
Kurosawa, J. Phys. Soc. Jpn. 16, 1298 (1961)
Multiple phonon modes(isotropic)
Anisotropic crystals
Amorphous materials and liquids
𝜀𝜀s𝜀𝜀∞
= �𝑖𝑖
𝑖𝑖𝐿𝐿𝑇𝑇,𝑖𝑖2
𝑖𝑖𝑇𝑇𝑇𝑇,𝑖𝑖2
det 𝜀𝜀sdet 𝜀𝜀∞
= �𝑖𝑖
𝑖𝑖𝐿𝐿𝑇𝑇,𝑖𝑖2
𝑖𝑖𝑇𝑇𝑇𝑇,𝑖𝑖2
Mathias Schubert, Phys. Rev. Lett. 117, 215502 (2016)
A.J. Sievers and J.B. Page, Infrared Physics 32, 425 (1991)
𝜀𝜀s𝜀𝜀∞
=𝑖𝑖2
𝑙𝑙
𝑖𝑖2𝑡𝑡
Infrared Lattice Vibrations (NiO)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 32
New Mexico State University
• Ni2+-O2- bonds are polar.• Ni-O vibration has dipole moment.
New Mexico State University
NiO or NaCl or LiF:Rocksalt lattice
FTIR ellipsometry
NiO
Typical Lorentz oscillator
𝜀𝜀 𝑖𝑖 = 𝜀𝜀∞ +𝐴𝐴𝑖𝑖0
2
𝑖𝑖02 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾0𝑖𝑖
Infrared Lattice Vibrations (NiO)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 33
•Rocksalt Crystal Structure (FCC), Space Group 225 (Fm-3m).
•Single TO/LO phonon pair.•Antiferromagnetic ordering along (111), should cause phonon splitting (8-30 cm-1).
•Second-order phonon absorption.
TO TA+TO phonon
NiO Reststrahlen Band
Rooksby, Nature, 1943
ε0=11.3ε∞=5.0
Willett-Gies & Nelson, JVST A 33, 061202 (2015)Also Humlicek PSSB 215, 155 (1999) for LiF.
NiO cell
Absorption in the restrahlen band
Two-phonon absorption (diamond)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 34
J.R. Hardy and S.D.Smith, Phil. Mag. 69, 1163 (1961)
A single photon excites two phonons. Energy and wave vector conserved.Two-phonon absorption is weak (lower probability than TO phonon absorption).Most likely to occur near Brillouin zone boundary (high density of states).
TA+LAO (X): 105+139=244 meV
Two-phonon absorption (GaP)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 35
E.S. Koteles, Solid State Commun. 19, 221 (1976)
Alternative to neutron scattering to determine zone-edge phonon energies.
Experiment
Theory
Phonons in complex oxides: Perovskites
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 36
5 atoms (SrTiO3), 4 optical phonons at Γ, 3Γ15(IR)+Γ25(silent)
Γ153Γ15
2
Loss function
TO3
LO2 LO3
Sr
Ti O
ε shows TO phonons
−1/ε shows LO phonons
Hard and soft phonons
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 37V.N. Denisov, Physics Reports 151, 1 (1987)
soft
hard Typical behavior: HardPhonon energy decreases with temperature.
Anomalous: SoftPhonon energy goes to zero at low temperature, drives a phase transition (collective movement of atoms)
SrTiO3 is nearly ferroelectric (TC~0 K).
𝜀𝜀s𝑖𝑖𝑇𝑇𝑇𝑇2 = 𝜀𝜀∞𝑖𝑖𝐿𝐿𝑇𝑇
2LST relation
𝑖𝑖TO → 0 at 𝑇𝑇𝐶𝐶 implies 𝜀𝜀𝑠𝑠 → ∞
Phonons in more complex oxides (bulk)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 38
Space Group
( ) ( )φχ cos2det += RNR R
63 or 3dD R cLaAlO3
7 or 3hO Fd mMgAl2O4
FTIR Ellipsometry
Loss function:LO phonons
Dielectric function: TO phonons
Willett-Gies, Thin Solid Films, 2013Zollner, Thin Solid Films, 2013
LO LO
TO TO
LaAlO3
MgAl2O4
3.03.222TO,
2LO, ±== ∏∞
i i
is ω
ωεε
2.08.72TO,
2LO, ±== ∏∞
i i
is ω
ωεε
Far-infrared ellipsometry (bulk LSAT)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 39
Disordered double perovskite (LaAlO3)0.3(Sr2AlTaO6)0.35Many phonon modes. Several reststrahlen bands.
ε shows TO phonons
−1/ε shows LO phonons
T.N. Nunley, JVSTA 34, 051507 (2016)
Phonons in more complex oxides (Co3O4 on spinel)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 40New Mexico State University
K.N. Mitchell, Kormondy, SZ, Demkov, JAP 115, 243708 (2014)
Cubic field splitting
Co3O4(22 nm)
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 41
Kramers-Kronig Relations
𝑃𝑃 𝑟𝑟, 𝑡𝑡 = 𝜀𝜀0 �𝜒𝜒𝑒𝑒 𝑟𝑟′ − 𝑟𝑟, 𝑡𝑡′ − 𝑡𝑡 𝐸𝐸 𝑟𝑟′, 𝑡𝑡𝑡 𝑑𝑑𝑡𝑡𝑡𝑑𝑑3𝑟𝑟𝑡
𝐷𝐷 𝑘𝑘,𝑖𝑖 = 𝜀𝜀0𝜀𝜀 𝑘𝑘,𝑖𝑖 𝐸𝐸 𝑘𝑘,𝑖𝑖
𝜀𝜀1 𝑖𝑖 − 1 =2𝜋𝜋℘�
0
∞𝑖𝑖′𝜀𝜀2 𝑖𝑖𝑡 𝑑𝑑𝑖𝑖′
𝑖𝑖′2 − 𝑖𝑖2
𝜀𝜀2 𝑖𝑖 = −2𝑖𝑖𝜋𝜋℘�
0
∞ 𝜀𝜀1 𝑖𝑖𝑡 𝑑𝑑𝑖𝑖′
𝑖𝑖′2 − 𝑖𝑖2
Response functionThe charges cannot move before the field has been applied.Kramers-Kronig relations follow:
𝜒𝜒𝑒𝑒 𝑟𝑟′ − 𝑟𝑟, 𝑡𝑡′ − 𝑡𝑡 = 0 for 𝑡𝑡′ > 𝑡𝑡
Contour integrals in complex plane:The real part of ε can be calculated if the imaginary part is known (and vice versa).Similar Kramers-Kronig relations for other optical constants.
�𝜒𝜒 𝑖𝑖𝑖𝑖′ − 𝑖𝑖
𝑑𝑑𝑖𝑖′ = 0
Cauchy
Analytical Properties of the Dielectric Function
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 42
Fields E(r,t) are real quantities
Onsager relationDielectric tensor symmetric (B=0)Also from energy density.Passive materials (no optical gain)
Like any analytic complex function, ε(ω) is defined by its zeroes and poles in the complex plane (below real axis). This implies
Works well for phonons and plasmons.
𝜀𝜀 −𝑘𝑘,−𝑖𝑖 = 𝜀𝜀 𝑘𝑘,𝑖𝑖𝜀𝜀 −𝑖𝑖 = 𝜀𝜀 𝑖𝑖
𝜀𝜀 −𝑘𝑘,𝑖𝑖 = 𝑡𝑡𝜀𝜀 𝑘𝑘,𝑖𝑖𝜀𝜀 𝑖𝑖 = 𝑡𝑡𝜀𝜀 𝑖𝑖
𝜀𝜀 𝑖𝑖 = 𝜀𝜀∞�𝑗𝑗=1
𝑁𝑁 𝑖𝑖LO,𝑗𝑗2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾LO,𝑗𝑗𝑖𝑖
𝑖𝑖TO,𝑗𝑗2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾TO,𝑗𝑗𝑖𝑖
R. P. Lowndes, PRB 1, 2754 (1970).
γ>0 (causality)
Also: Berreman & Unterwald, Phys. Rev. 174, 791 (1968); Zollner, JVST B (2019).
𝜀𝜀2 𝑖𝑖 ≥ 0
Comparison of Lorentz and Lowndes Models
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 43
Drude-Lorentz Model
Lowndes Model
Drude terms: Poles on the imaginary axis (ω0=0)Additional broadening parameter for LO phonon.Lorentz identical to Lowndes model, if ωTO=ωLO.Otherwise: Frictional force allowed to vary with velocity. Complex Lorentz amplitude, frequency-dependent damping.Lowndes model makes no assumptions about forces.
𝜀𝜀 𝑖𝑖 = 𝜀𝜀∞�𝑗𝑗=1
𝑁𝑁 𝑖𝑖LO,𝑗𝑗2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾LO,𝑗𝑗𝑖𝑖
𝑖𝑖TO,𝑗𝑗2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾TO,𝑗𝑗𝑖𝑖
R. P. Lowndes, PRB 1, 2754 (1970).
𝜀𝜀 𝑖𝑖 = 1 −�𝑖𝑖
𝑖𝑖𝑃𝑃,𝑖𝑖2
𝑖𝑖2 + 𝑖𝑖𝛾𝛾𝐷𝐷,𝑖𝑖𝑖𝑖+ �
𝑖𝑖
𝐴𝐴𝑖𝑖𝑖𝑖0,𝑖𝑖2
𝑖𝑖0,𝑖𝑖2 − 𝑖𝑖2 − 𝑖𝑖𝛾𝛾0,𝑖𝑖𝑖𝑖
Berreman & Unterwald, Phys. Rev. 174, 791 (1968).
Summary
Stefan Zollner, February 2019, Optical Properties of Solids Lecture 6 44
• Drude model explains optical response of metals.• High reflectance below the plasma frequency.• Interband transitions overlap with Drude absorption.
• Doped semiconductors have infrared plasma frequencies.
• Lorentz model explains infrared lattice absorption.• TO/LO modes result in reststrahlen band.• Multiple modes for complex crystal structures.